Enhanced detection of low concentration volatile organic compounds using advanced doped zinc oxide sensors

Pure zinc oxide nanoparticles, as well as those doped with 3% calcium, aluminum, and gallium, were synthesized using a sol–gel method and then deposited onto an alumina substrate for sensing tests. The resulting nanoparticles were characterized using a variety of techniques, including X-ray diffraction (XRD), scanning electron microscopy (SEM) equipped with energy dispersive X-ray analysis (EDX), transmission electron microscopy (TEM), UV-VIS-NIR absorption spectroscopy, and photoluminescence (PL) measurements, to examine their structural, morphological, and optical properties. The prepared nanoparticles were found to have the hexagonal wurtzite structure of ZnO with a P63mC space group. The UV-Vis-IR spectra showed that the samples are highly absorbent in the UV range, while the PL spectra confirmed the presence of many defects in the ZnO structure, such as oxygen vacancies and zinc interstitials. The doped samples exhibited more defects than the pure sample. SEM images of the deposited film surface showed agglomerates with a spherical shape and confirmed the nanometer scale size of our prepared samples, as corroborated by the TEM images. The EDX spectra indicated the high purity of the ZnO deposited films, with a high presence of Zn and O and the presence of the doped elements (Ca, Al, and Ga) in each doped sample. Sensing tests were performed on ZnO, Ca3%-doped ZnO (C3ZO), Al3%-doped ZnO (A3ZO), and Ga3%-doped ZnO (G3ZO) sensors in the presence of volatile organic compounds (VOCs) gases such as ethanol, formaldehyde, methanol, and acetone at low concentrations. The sensors exhibited high responses to low ppm level concentrations of the VOCs gases. At a low operational temperature of 250 °C, the C3ZO sensor had the highest response to 5 ppm of ethanol, methanol, and formaldehyde gases compared to the pure and other doped sensors. Additionally, the A3ZO sensor exhibited the highest response to acetone gas. In conclusion, our findings suggest that the doping of zinc oxide can enhance the low concentration detection of VOCs gases, with the C3ZO and A3ZO sensors showing the highest response to specific gases.


Introduction
Air pollution is a global problem in our world caused by the development of industry.Every year, three million people die due to environmental pollution, and according to recent statistics, this number could grow to more than six million by 2050 if the same trend in pollution emission levels continues. 1To see a solution to this problem, several researchers have been studying the construction of devices that allow the detection of toxic gases.
Metal oxide-based gas sensors (MOX) are a technology that has attracted great attention in several elds, such as solar cells, electrical assemblies, gas sensors, etc. MOX have several important characteristics, such as being low cost, easy to use, and highly sensitive to various gases. 2,3The detection of volatile organic compounds (VOCs) is essential in industry and in the laboratory environment.VOCs in the human breath, such as acetone, ethanol, ammonia, ethane, and pentane, serve as biomarkers for several diseases. 4Typical levels of acetone in the breath of healthy RSC Advances PAPER humans range from 0.3 to 4 ppm, 5,6 while this can increase to 40 ppm in adults that follow a ketogenic diet. 7In addition, there are other types of VOCs, such as methanol and formaldehyde, which can negatively affect human health.For example, exposure to a concentration of formaldehyde greater than 6 ppm can cause nasopharyngeal cancer, leukemia, and even lung cancer. 8Also, methanol is very toxic and oen fatal to humans. 9as sensors based on semiconductor metal oxides (MOS) are the most promising because of their compact design, their low cost, their high sensitivity, and their applicability in the detection of VOCs in expired air.Most sensor materials, such as In 2 O 3 , 10 SnO 2 , 11 Fe 2 O 3 , 12,13 ZnO, 14 WO 3 , 15 TiO 2 , 16 Co 3 O 4 , 17 and so on, have excellent gas detection properties.In particular, there are several reports where chemoresistive sensors, based on metal oxides, have been used for the detection of VOCs.Zinc oxide, which has several interesting properties, is a type II-VI semiconductor material with a high exciton binding energy of ∼60 meV and a wide band gap of 3.37 eV.As such, zinc oxide has received considerable attention due to its many applications in optoelectronics, gas sensors, solar cells, and electronics. 18,19Also, compared to other metal oxides, ZnO is quite attractive for its high thermal and chemical stability and its relatively simple preparation.The detection properties of sensors based on ZnO can be modulated by altering the particle morphology, crystal structure, and energy band structure.Li et al. 20 report that a gas sensor based on ZnO nanowalls has a high acetone vapor detection response with rapid recovery and response times.Jaballah et al. 21showed that Ca-doped ZnO nanopowder elaborated via a sol-gel method has good formaldehyde sensing properties with a high response rate (5 ppm, 250 °C) and a low detection limit at each ppm concentration they examined.Zahmouli et al. 22 proved that a sensor based on g-Fe 2 O 3 /Al-ZnO nanocomposites, prepared using a sol-gel method, had a high sensitivity to acetone gas.
In this work, we present a study of the sensing properties of pure and doped ZnO materials in response to low concentrations of VOCs gases.The prepared samples were made using a modied sol-gel process.The zinc oxide was doped with aluminum, calcium, and gallium to enhance its sensing performance.The VOCs gases tested were acetone, methanol, ethanol, and formaldehyde.Structural, morphological, and optical proprieties were investigated to explain the sensing mechanism.

Synthesis of ZnO nanoparticles and characterization
A sol-gel method was used to synthesize the ZnO nanoparticles.We dissolved 16 g of zinc acetate dihydrate [Zn(CH 3 COO) 2 , 2H 2 O, 99%] in 112 mL of methanol.The solution was maintained under magnetic stirring until the precursor was dissolved.Then, we introduced the solutions into an autoclave with 220 mL of ethyl alcohol to dry the solution under the supercritical conditions of ethanol (T c = 243 °C, P c = 63.6 bar).The resulting powder was calcined in a muffle furnace under air at 400 °C for 2 hours.
Structural and morphological characterizations of the prepared samples were carried out using a Philips PW1710 X-ray diffractometer with CuKa1 radiation (1.54186 Å) and using eldemission scanning electron microscopy (FE-SEM, S4800II, Hitachi, Japan) with energy dispersive X-ray analysis (EDX).Transmission electron microscopy (TEM) was performed using a JEOL JEM 2010 electron microscope (LaB6 electron gun) equipped with a Gatan 794 Multi-Scan CCD camera and operating at 200 kV.A NanoLog Horiba modular spectrouorometer was used to conduct the photoluminescence (PL) measurements to understand the optical properties and to investigate the defects found at the bandgap of the nanomaterial.The excitation light source used was a Xe lamp.The range of emission was between 350 and 750 nm at an excitation wavelength of 325 nm.Also, the UV-vis absorbance spectra were acquired using a UV-vis spectrophotometer (Shimadzu UV-3101PC).

Sensor fabrication and sensing tests
250 mg of the prepared nanopowder was dissolved in 2.25 mL of distilled water.Then, the mixture was sonicated by ultrasound until a uniform and dispersed solution was obtained.Subsequently, we deposited the homogeneous solution on alumina substrates (Al 2 O 3 ) (C-MAC Micro Technology Company, Belgium) equipped with a pair of interdigitated gold electrodes and Pt heating elements, by a spray method.To stabilize the deposited lm on the substrate, the sensor was heated for 1 hour at 400 °C.
Detection tests were performed in a homemade gas detection measurement system.We begin by injecting commercial synthetic air (79% N 2 + 21% O 2 ) into a Teon chamber, which contains the sensor being tested, until the baseline is stable.Aer that, we inject the target gas at an appropriate concentration.The relative humidity (RH) and temperature were continuously monitored.The gas sensor response is dened as S = R a /R g where R a and R g are the electrical resistance of the sensor in air and the target gas, respectively.Response/recovery times were evaluated at the 90% resistance change point aer exposure to the target gas and air.

Structural properties
The crystallographic structures of the prepared samples of ZnO, Ca 3% -doped ZnO (C3ZO), Al 3% -doped ZnO (A3ZO), and Ga 3%doped ZnO (G3ZO) were obtained via X-ray diffraction analysis at room temperature, as presented in Fig. 1-a-d, respectively.All spectra were rened by the Rietveld method using the FullProf soware.This method is based on the pseudo-Voigt function.The renement indicates that all samples crystallize in the hexagonal structure with the P63mC space group.This indicates that doping with Ca, Al, and Ga does not induce a structural change in the ZnO structure.In addition, no distinct phase is observed in our samples.All tting parameters are collected in Table 1 and the excellent goodness of t, c 2 , values indicate the good quality of the renement.There is good agreement between the observed and the calculated plots.
The plots of (b cos q) versus (4 sin q) were tted according to eqn (1).The D value is estimated from the slope of the extrapolation of the linear t and the 3 value is given by the t slope.The obtained D values are equal to 52 nm, 126 nm, 37 nm, and 30 nm for the ZnO, C3ZO, A3ZO, and G3ZO samples, respectively.The obtained results show that doping with calcium increases the grain size more than doping with the other elements due to the difference in size of the radii of Ca 2+ (r = 99 pm) and Zn 2+ (r = 74 pm).Meanwhile, the smaller radii of Ga 2+ (r = 62 pm) and Al 3+ (r = 53 pm) cause a reduction of the crystallite size.In addition, the dislocation density (d) was calculated using the following relationship: The calculated values of D, 3, and d of the prepared samples are presented in Table 1.The high observed values of d, present essentially in the doped samples, suggests that there are defects present in the structure of the prepared samples.These defects can improve the gas detection performance of the samples.

Morphological proprieties
The typical SEM micrographs of our samples ZnO, C3ZO, A3ZO, and G3ZO are displayed in Fig. 2-a-d, respectively, and show the surface morphology and the distribution of the grain size (D).The obtained pictures show the presence of agglomerates with a spherical form with an uneven distribution.The insets of Fig. 2 illustrate the Gaussian-tted histograms calculated using the ImageJ soware.The histograms indicate the distribution of average grain size in our samples.The average grain sizes determined by SEM are equal to 38, 68, 23, and 35 nm for ZnO, C3ZO, A3ZO, and G3ZO, respectively.All grain size values are collected in Table 1.The particle size values estimated from SEM are larger  than those estimated from the W-H formula.Each grain is almost monocrystalline in nature.The SEM images show a smaller grain size for A3ZO, and G3ZO and larger grain sizes for C3ZO, thus conrming the observations obtained from the W-H method.Fig. 2-e-h present TEM images of the particle shapes of the ZnO, C3ZO, A3ZO, and G3ZO samples, respectively.The grain sizes, as evidenced by the TEM of the prepared samples, agree well with the SEM images and are less than 100 nm, thus conrming the nanometer scale of the prepared powders.The shapes of almost all the particles are spherical with the presence of some hexagonal nanoparticles also noted.Fig. 3-a-d show the EDX spectra of the ZnO, C3ZO, A3ZO, and G3ZO samples, respectively.This method is used to determine the purity and to conrm the presence of the constitutional elements in our samples.The EDX spectra prove the presence of all elements, such as Zn, O, Ca, Ga, and Al, in our compounds.It is worth noting that no constitutional elements were lost in our samples compositions.In addition, we note the presence of carbon and aluminum in the spectra.The carbon comes from the precursor compound and the aluminum from the sensor substrate.

Photoluminescence and UV-visible light absorption characterization
The PL spectra of the doped and pure ZnO samples were captured and are shown in Fig. 4-a.Pure zinc oxide has a large peak in the visible light region resulting from a deep-level emission (DLE), as well as a peak in the UV region that is focused on a near band edge (NBE) emission.The large visible band is linked to several intrinsic defects.Ca doping causes the NBE peak to move to shorter wavelengths, which may be related to the Moss-Burstein effect.The Fermi level and optical band gap are oen increased in C3ZO nanostructures due to the replacement of the Zn 2+ ions that are present in their network locations with Ca 2+ ions.Ca doping induces a sharp rise in emission intensity.This is mostly due to the Ca 2+ ions, which have a larger atomic radius (1.14 Å) than zinc ions, replacing Zn 2+ ions, which have a smaller atomic radius (0.88 Å).The sites in the crystal structure are disrupted by this substitution, which also increases the number of defects present in the substance.This leads to an increase in the number of oxygen defects (V o ), which has been linked to green emissions, and an increase in the number of interstitial zinc sites (Zn i ), which has been linked to red emissions. 25,26eyond that, there were visual differences between the PL emission spectra of the pure ZnO and Al-doped ZnO (A3ZO) samples.The UV emission band intensied while the green emission band steadily diminished in intensity.A new band with a center at 437 nm also developed, which we relate to a blue emission.This emission may result from intrinsic aws or from the recombination of donor-acceptor pairs linked to the acceptor Al.Overall, our ndings indicate that the strength of the blue band grew as the Al content increased, whereas the intensity of the green band decreased as the Al content increased. 27Ga-doped ZnO (G3ZO) exhibits a dramatic reduction in its green emission and an increase in the UV emission in its PL spectrum.Ga atoms occupy Zn vacancy defect positions and increase the donor-associated defect amounts in ZnO, resulting in intense UV emissions in the PL spectra. 28he absorbance spectra of ZnO, C3ZO, A3ZO, and G3ZO in the UV-visible-NIR range were examined and are displayed in Fig. 4-b.It was found that the absorbance decreased noticeably for wavelengths higher than 400 nm (in the visible and near infrared ranges) and that the absorbance was highest in the UV light range (400 nm).Such a redshi in the photosensitivity of the Ca-doped ZnO sample presumably resulted from the subband gap transitions produced by the incorporation of the Ca ions in the structure of ZnO, as evidenced by an absorption wavelength of the Ca-doped ZnO nanoparticles of 400-500 nm.According to the UV-vis absorption spectrum of A3ZO, the edge values of the AZO nanoparticles were blue-shied in comparison to the ZnO nanoparticles, and the absorbance in the visible region improved primarily as a result of the deep levels in the ZnO bandgap caused by an increased concentration of defects. 2 Ga doping makes it possible to increase the optical absorption rate in the visible range, thus revealing that the light absorption capacity is increased by the intercalation of the gallium atoms, resulting in easier transport of the charge carriers between the valence and conduction bands.
In order to determine the band gap energy of the prepared samples, the variation of (ahy) 2 as a function of the energy of the photons was studied (Fig. 4-c) according to Tauc's model: ( Here, a, h, n and A are the absorption coefficient, the Planck constant, the photon frequency, and a constant, respectively.For materials with a direct band gap, the exponent "n" has a value of 1/2.The band gap energy (E g ) for each sample can be calculated by extrapolating the linear portion of the curve to the x-axis.For ZnO, C3ZO, A3ZO, and G3ZO, the estimated E g values are 3.22, 3.18, 3.21, and 3.19 eV, respectively.We see that the E g According to published research, a decrease in the energy of the band gap can be attributed to a drop in carrier concentration, an increase in tensile stress, and an increase in inter-band defects such oxygen vacancies. 29

Gas sensing performance
The prepared sensors were tested in the presence of 5 ppm of acetone, ethanol, methanol, and formaldehyde gases with 50% RH at different temperatures ranging from 200 to 350 °C.The sensor responses to VOCs gases, such as acetone, ethanol, methanol, and formaldehyde, as a function of temperature are presented in Fig. 5-a-d, respectively.The curves indicate that the highest responses are at an operational temperature of 250 °C.
The doped sensors present a response to VOCs gases better than the pure sample.The best response to acetone gas came from the A3ZO sensor and the best sensor response to ethanol, methanol, and formaldehyde gas came from the C3ZO sensor.In addition, we note that doping ZnO with Ga enhances the response to acetone gas.This improvement is related to doping in general because it creates defects in the internal structure of the ZnO.These defects are generally interstitial and oxygen vacancies, which have the most important role in the gas detection mechanism. 30The improved acetone gas responsiveness of the A3ZO sensor may be attributed to the following factors.First off, the A3ZO NPs have a smaller size than the ZnO NPs and a nanospherical structure, factors which both point to a larger specic area.Gas molecules will diffuse more readily as a result, and they will interact with the adsorbed oxygen on the A3ZO surface more positively.This implies that it may be possible to signicantly increase the concentration of adsorbed species.Secondly, the presence of oxygen vacancies, whose adsorption energy is probably three times greater than that of the optimal position, could have a major impact on the sensor response. 31Unoccupied oxygen sites in the A3ZO structure are utilized as an adsorption site to improve gas detection.As a result, gas molecules can react with oxygen species that have been adsorbed at open oxygen sites.When there are several gas molecules adsorbed on the surface, there is a lot of electron mobility.Despite the electron ow remaining unaltered, this causes the percolation channel to widen and the electrondepleted layer to contract.The electrical resistances of the prepared sensors in the presence of ethanol, methanol, formaldehyde, and acetone gas at different gas concentrations at 250 °C and under a humidity of 50% are presented in Fig. 6-a-d, respectively.We investigated the sensor response to various low concentrations of each gas (1 ppm, 2.5 ppm, and 5 ppm) to see what effect low VOCs gas concentrations had on the sensor responses.Each concentration was injected two times consecutively to understand the reproducibility of our sensors.The responses to each concentration are almost consistent for all gases which indicates the high reproducibility of our sensors to low ppm concentrations of VOCs gases.Note that for the prepared sensors, upon exposure to the target gas, the resistance decreased rapidly to an equilibrium level and then it returned to baseline when humid air was reinjected into the Teon chamber.This behavior is in good agreement with the behavior associated with the detection mechanism of n-type semiconductors.At an operating temperature of 250 °C, we conducted comparisons between all the sensors that were investigated.This highlighted that the Ca-doped ZnO nanoparticles have excellent potential for detecting ethanol, methanol, and formaldehyde fumes at low concentrations.It is evidently true that aer each pulse, the signal of the Ca-doped lms resets to its initial value.This behavior demonstrates the reversibility of the surface layer adsorption of the tested gases.The baseline resistances of the Ca-doped ZnO sample are higher than those of the undoped ZnO, it should be noted.The decrease in the carrier concentration of the Ca-doped sample is associated with this rise in resistance.As opposed to the other sensors based on doped samples, the baseline resistance of the Ca-doped ZnO sample increases following Ca doping by 3%, indicating a larger baseline resistance.The increased resistance may be primarily responsible for the higher responsiveness of the C3ZO sensor.The increased resistance is most likely due to the many aws on the surface, which allow for the chemisorbtion and ionized adsorption of numerous oxygen molecules.The sensor response and baseline resistance both follow the same pattern.As more Ca is inserted, they grow.Particularly at low gas concentrations, C3ZO has ethanol, methanol, and formaldehyde detecting abilities that are competitive in comparison to other literature studies.High basicity is an attribute of calcium and on the surface of ZnO it produces centers with simple character.The high adsorption of the tested gases is facilitated by these sites, and therefore the good sensing performance was caused by the Ca doping.Therefore, C3ZO could be helpful for the creation of a highefficiency ethanol, methanol, and formaldehyde gas sensor for real-world applications due to its straightforward synthesis process and outstanding gas detection capabilities.
The response/recovery times were estimated from the base resistance variation of the pure and doped ZnO samples in response to air and the target gases.Fig. 7-a-d present the resistance as a function of time in response to air and the target gases (acetone, ethanol, methanol, and formaldehyde) at a concentration of 5 ppm at 250 °C and at 50% RH, for ZnO, C3ZO, A3ZO, and G3ZO, respectively.By comparing the pure and doped samples, we can see that the doped samples have faster response and recovery times than pure ZnO.This behavior can enhance the efficacity of sensors.Thus, doping improves the most important parameters (responses and response/recovery times) required for gas detection.
Selectivity is a parameter that describes the capacity of a sensor to distinguish between particular input signals.For sensors operating in complicated settings, selectivity is crucial. 32By observing the reaction of a transmitter to a specic gas concentration, we may calculate selectivity.This response is the same as the sensor response brought on by a certain target gas concentration.Cross-sensitivity lowers the measurement repeatability and reliability, making this attribute crucial for monitoring numerous gas applications.Good sensitivity and high selectivity are necessary for the perfect sensor.To increase selectivity, modied layer and gas sensor arrays are integrated.The selectivity diagrams of the pure and doped ZnO sensors are presented in Fig. 8-a and show the sensor responses towards 5 ppm of acetone, ethanol, methanol, and formaldehyde gas at 250 °C and at 50% RH.Pure ZnO has a higher selectivity for ethanol gas compared to the other tested gases.Also, we note that the C3ZO sensor presents a higher selectivity for ethanol than the other gases and that its selectivity to acetone gas is marginally smaller than its selectivity to ethanol.
The A3ZO sensor has a better sensitivity toward acetone vapor than to formaldehyde, ethanol, and methanol, showing superior acetone vapor selectivity.By including Al in the ZnO structure, the reaction to acetone is enhanced while the reactivity to formaldehyde, ethanol, and methanol is minimized.The extraordinary selectivity of the Al-doped ZnO nanoparticles may be attributed to the difference in the dipole moments of the target gases, which is signicantly greater for acetone (2.91 D) than for ethanol (1.66 D), methanol (1.70 D), and formaldehyde (2.33 D).Other factors, such as the size and molecular weight of the gas molecules, also affect how the sensor responds. 33

Gas sensing mechanism
Oxygen adsorption and desorption on the ZnO deposit layers have been demonstrated experimentally by exposure to humid air at a working temperature ranging from 200 °C to 350 °C.The interaction of atmospheric oxygen with the ZnO surface forms a layer of charged oxygen species which traps electrons from most of the material.The electrons captured during this process are removed from the conduction band and conned in the adsorbed oxygen species at the surface. 34Therefore, a space charge zone is formed because the presence of negative surface charges leads to web bending dened by a potential barrier to the surface.This restricts the weak electrons and subsequently allows a decrease in conductivity.
Fig. 6 shows a change in resistance during alternate exposure to moist air and organic vapor (ethanol, formaldehyde, methanol, and acetone) at different concentrations.These measurements were carried out at an optimal temperature of 300 °C.The evolution of the response as a function of the working temperature shows an optimum temperature for each gas.There is a direct correlation between oxygen adsorption and the detection of the reducing gas.In fact, the responses to the reducing gases exhibit a similar evolution and neighboring optimum temperatures.Increasing the operating temperature under the optimum temperature improves the oxygen adsorption and therefore the response to VOCs.In contrast, the desorption of all previously adsorbed ionic oxygen species occurs at high temperatures, which explains the decrease in the response to reducing gases above the optimum temperature.
For the identication of the ionosorption of oxygen species, we performed measurements on the ZnO sensor at an operating temperature of 250 °C by varying the concentrations of ethanol, formaldehyde, methanol, and acetone.Thus, the adsorbed oxygen ionization equations can be written by the following equations: O 2(ads) + 4e − / 2O (ads) 2− . ( When we inject a reducing gas into the tested cell, the molecules of the gas will react with the oxygenated species on the surface of the material which causes a reinjection of electrons in our detection material and subsequently the potential barrier will be reduced and the conductivity will be increased.The reactions between the VOCs gases (ethanol, formaldehyde, methanol, and acetone) and the oxygen species are expressed by the following equations: The general reaction between the oxygen species and the main element of the reducing gas is shown in more detail in the mechanism presented in Fig. 8-b.

Comparative study of prepared samples vs. other materials
To evaluate the performance of our prepared samples in comparison to other materials, we conducted a comprehensive analysis by referencing the literature on the responses of other materials to VOCs, specically acetone, ethanol, methanol, and formaldehyde.We considered key parameters such as operational temperature and gas concentration, which are detailed in Table 2.
Our most effective sensor for detecting acetone gas was found to be ZnO doped with 3% Al, exhibiting superior sensing characteristics when compared to other sensors based on ZnO.

Conclusions
Pure and doped zinc oxide powders were prepared via a sol-gel route and were characterized using X-ray diffraction (XRD), scanning electron microscopy (SEM) equipped with energy dispersive X-ray analysis (EDX), transmission electron microscopy (TEM), UV-VIS-NIR absorption spectroscopy, and photoluminescence (PL) measurements.The prepared samples had the hexagonal wurtzite structure of the ZnO material.We have sprayed the synthesized powders on an alumina substrate.The SEM images of the deposited lms showed agglomerates with a spherical shape which conrmed the nanometer scale size of our samples whilst the EDX spectra indicated the high purity of the ZnO deposited lm.The EDX analysis also showed the presence of the doping elements Ca, Al, and Ga in the structures of the Ca 3%doped ZnO (C3ZO), Al 3% -doped ZnO (A3ZO), and Ga 3% -doped ZnO (G3ZO) samples.The UV-Vis-IR spectra indicate a high absorption in the UV range and the estimation of the band gap energies indicates values that range from 3.18 to 3.22 eV where the highest value relates to the pure sample and the lowest value relates to C3ZO, indicating that doping can create a defect inter-band.The PL spectra indicated the presence of a peak in the UV region that is focused on a near band emission (NBE) (deep-level emission) and a large visible band linked to several intrinsic defects in our structure, such as Zn interstitial (Zn i ) and oxygen vacancies (V o ).Ca doping caused the NBE peak to move to shorter wavelengths which is related to the Moss-Burstein effect.A3ZO presents an intensied UV emission band while the green emission band steadily diminished in intensity.G3ZO exhibits a reduction in the green emission and an increase in UV emission.We have investigated the VOCs (ethanol, formaldehyde, methanol, and acetone) sensing capabilities of the elaborated sensors at low concentrations.The sensors exhibit a high response to low ppm concentrations of VOCs gases at a low operational temperature of 250 °C and at a humidity of 50%.Doping ZnO with Ca enhances the

Fig. 1 -
f represents the Williamson-Hall plots.The micro-deformation (3) and the average size of the crystallites (D) were estimated according to the Williamson-Hall model: 23

Fig. 5
Fig. 5 Sensor responses as a function of temperature in the presence of 5 ppm of (a) acetone, (b) ethanol, (c) methanol, and (d) formaldehyde gases for the ZnO, C3ZO, G3ZO, and A3ZO samples.

Fig. 6
Fig. 6 Electrical resistance versus time for the ZnO, C3ZO, A3ZO, and G3ZO sensors at 250 °C and under 50% RH in response to (a) acetone, (b) ethanol, (c) methanol, and (d) formaldehyde gas at different concentrations.

Fig. 7
Fig. 7 Base resistances as a function of time in response to acetone, ethanol, methanol, and formaldehyde gas for the (a) ZnO, (b) C3ZO, (c) A3ZO, and (d) G3ZO sensors.

Fig. 8
Fig. 8 (a) Sensors responses towards 5 ppm of the target gases at 250 °C and at 50% RH.(b) Schematic of the gas sensing process under air and reducing gas atmospheres.

Table 2
Comparison of VOCs (acetone, ethanol, methanol, and formaldehyde) gas-sensing performance of sensors in this study with other materials , methanol, and formaldehyde gases and doping ZnO with Al ameliorates the sensitivity to acetone gas with an increased selectivity to this gas.